reduction reaction (ORR), or anchor the metal nanoparticles
used in the catalytic reaction. Moreover, after nitrogen doping
in the monolayer graphene, the Fermi level shifts above the
and the density of state near the Fermi level is
thus, the band gap between the conduction
band and the valence band will be opened. For GNRs, the band
gap is still kept after doping.31
The band gap in N-graphene
makes it a candidate to be used in semiconductor devices. Apart
from these, N-graphene can also be used in batteries, sensors,
and ultracapacitors. The nitrogen doping of graphene greatly
broadens its applications.
Previously, several reviews on graphene have mentioned N-
especially the review of Liu et al.,35
focused on two chemical doping approaches and band gap
tuning; however, there is still no systematical study of N-
graphene synthesized by substitutional doping. Therefore, in
this review, we summarize diﬀerent synthesis and character-
ization methods of nitrogen-substituted graphene; the
application of N-graphene is also reviewed on the basis of
experimental and theoretical studies.
2. SYNTHESIS OF N-GRAPHENE
Similar to the synthesis of N-CNT, N-graphene can be
obtained through two diﬀerent ways: direct synthesis and
post treatment. Most postsynthesis treatments may lead to
surface doping only. Although in principle, direct synthesis may
have the potential to create a homogeneous doping throughout
the bulk material, the results reported so far fail to indicate so.
Speciﬁcally, direct synthesis includes chemical vapor deposition
(CVD), segregation growth, solvothermal, and arc-discharge
approaches. Post treatment includes thermal treatment, plasma
treatment, and N2H4 treatment. Table 1 gives a summary of
various methods used for the synthesis of N-graphene. Detailed
discussion on these methods is elaborated below.
2.1. Direct Synthesis. 2.1.1. CVD Approach. CVD is a
widely used method to synthesize various carbon nanomateri-
als, such as graphene,36
Recently, it was successfully applied to prepare
a metal catalyst (Cu or Ni) is
used as the substrate, then at high temperature, a carbon source
gas mixed with a nitrogen-containing gas is introduced. These
precursors dissociate and recombine into N-graphene by means
of precipitation on the surface of the catalyst.30,42
Apart from the gas mixture, liquid organic precursors
(acetonitrile, pyridine) have also been used to form N-
Theoretical study about diﬀerent precursors45
shows that proper skeletal bonds of liquid precursors are crucial
for the formation of N-graphene. Acrylonitrile containing the
C−C single bond, CC double bond, and CN triple bond
cannot form N-graphene, but pyridine with only the double
bond forms N-graphene. The proposed reason is that the single
bond is easy to break, even at low temperature, leaving CC
and CN bonds at the catalyst surface. Then CN bond is
Table 1. Nitrogen-Doping Methods and Nitrogen Concentration on Graphene
method precursors N content, at. %
1 CVD Cu ﬁlm on Si substrate as catalyst, CH4/NH3 1.2−8.9 FET30
2 CVD Cu foil as catalyst, NH3/He 1.6−16 ORR40
3 CVD Ni ﬁlm on SiO2/Si substrate as catalyst, NH3/CH4/H2/Ar (10:50:65:200) 4 ORR41
4 CVD Cu foil as catalyst, acetonitrile ∼9 lithium battery43
5 CVD Cu foil as catalyst, pyridine ∼2.4 FET44
carbon-contained Ni layer on nitrogen-contained boron layer 0.3−2.9 FET50
7 solvothermal Li3N/CCl4 (NG1) or N3C3Cl3/Li3N/CCl4 (NG2) 4.5 (NG1) or 16.4 (NG2) ORR52
8 arc discharge graphite/H2/He/pyridine (NG1) graphite/H2/He/NH3 (NG2) transformation of
0.6 (NG1), 1 (NG2), 1.4
ion-irradiated graphene, NH3 1.1 FET59
graphite oxide after thermal expansion, NH3/Ar 2.0−2.8 ORR60
GNR, NH3 FET31
GO, NH3/Ar (10% NH3) ∼3−5 FET63
GO, NH3 6.7−10.78 methanol
GO, melamine 7.1−10.1 ORR62
graphite oxide after thermal expansion, N2 plasma 8.5 ORR23
graphite oxide after thermal expansion, N2 plasma 3 ORR67
chemically synthesized graphene, N2 plasma ∼1.3 biosensors68
GO, treat with H2 plasma ﬁrst, then treat with N2 plasma 1.68−2.51 ultracapacitor69
mechanically exfoliated graphene or bilayer graphene grown by CVD, NH3 plasma FET70
GO, N2H4, NH3 4.01−5.21 71
graphite oxide after thermal expansion, N2H4 1.04 electrochemical
ACS Catalysis Review
dx.doi.org/10.1021/cs200652y | ACS Catal. 2012, 2, 781−794782
preferentially removed from the surface by forming volatile
molecules when the temperature is higher than 400 °C; thus,
only CC will be left to form nondoped graphene above 500
°C. In contrast, the skeletal bonds in pyridine have similar bond
energies, which induces the formation of N-graphene.
The layer distribution of N-graphene is varied in diﬀerent
studies. Although the N-graphene synthesized from the gas
mixture C2H4/NH3 is claimed to be monolayer through the
analysis of Raman spectroscopy,40
from a gas mixture, CH4/NH3,30,41
shows that the few-layer
graphene is predominant after high-resolution transmission
electron microscope (HRTEM) characterization. In other
studies, monolayer N-graphene is also obtained when
is used as precursors. Furthermore,
the layer of N-graphene can be adjusted by the ﬂowing time if
acetonitrile is used as the precursor.43
In the CVD approach, the nitrogen content can be controlled
by changing the ﬂow rate40
and the ratio between carbon
source and nitrogen source.30
It has been reported30
doping level decreased from 8.9 to 3.2 or 1.2 at. % if the NH3/
CH4 ratio was lowered from 1:1 to 1:2 or 1:4, respectively.
Moreover, although high nitrogen content (∼16 at. %) has
the nitrogen content in this method is
normally around 4−9 at. %.
The bonding conﬁguration of nitrogen within N-graphene
varies with diﬀerent studies. By using Cu as the catalyst and
CH4/NH3 (1:1) as the precursor, the nitrogen type in N-
graphene is mainly quaternary N;30
however, when Ni is used
as the catalyst and CH4/NH3 (5:1) is used as the precursor, the
obtained N-graphene consists of mainly pyridinic N and
If C2H4/NH3 is used as the precursor while
keeping Cu as the catalyst, the pyridinic N becomes the
Notably, the syntheses of other nitrogen-
doped carbon materials have revealed that the doping
environment is also inﬂuenced by the ﬂow rate, catalyst, and
so further research is required to
clarify the relationship between the bonding conﬁguration of
nitrogen and the parameters of CVD.
2.1.2. Segregation Growth Approach. In this approach, a
nitrogen-containing boron layers and carbon-containing nickel
layers are sequentially deposited on the SiO2/Si substrate by
electron beam evaporation, then during the vacuum annealing
process, the boron atoms are trapped by nickel, and the carbon
atoms will segregate out onto the nickel surface and combine to
form N-graphene (Figure 2).50
Although sporadic multilayer
areas are observed, the N-graphene generally shows a large-
scale, uniform, and few-layer structure. The nitrogen content
(0.3−2.9 at. %) can be controlled by adjusting the thickness of
the boron and nickel ﬁlms. The pyridinic and pyrrolic N are
dominant in N-graphene. Interestingly, the graphene can be
doped in a speciﬁc area by embedding nitrogen species into the
selective area of the substrate.
2.1.3. Solvothermal Approach. The solvothermal approach
was ﬁrst employed for gram-scale production of graphene.51
Recently, gram-scale production of N-graphene has been
achieved by applying this approach at ∼300 °C. By mixing
lithium nitride (Li3N) with tetrachloromethane (CCl4) (Figure
3) or cyanuric chloride (N3C3Cl3) with Li3N and CCl4, N-
graphene with diﬀerent nitrogen contents was obtained
(denoted as NG1 and NG2, respectively).52
images of N-graphene show that it mainly consists of 1−6 layer
graphene. Because of the introduction of N3C3Cl3, NG2 has a
higher nitrogen content (16.4 at. %) compared with NG1(4.5
at. %). The proportion of doped nitrogen species also changes
with diﬀerent reactant mixtures. The quaternary N dominates
in NG1, and pyridinic and pyrrolic N dominates in NG2.
2.1.4. Arc-Discharge Approach. An arc-discharge approach
has been applied to obtain CNTs and doped CNTs by
evaporating the carbon source, normally graphite,53−55
temperature. Rao et al.56,57
successfully obtained N-graphene
by applying this method in the presence of pyridine vapor or
NH3. The N-graphene synthesized from transformation of
nanodiamond shows higher nitrogen content than that
synthesized from graphite. The nitrogen content of the as-
synthesized N-graphene is around 0.5−1.5 at. %. Moreover,
although single layer N-graphene is occasionally observed, most
of the N-graphene possesses two or three layers. The scale of
graphene and N-graphene produced by this method normally is
below 1 μm.56,58
2.2. Postsynthesis Treatment. 2.2.1. Thermal Treat-
ment. Thermal treatment refers to the method using high
temperature to produce N-graphene. It has been shown that
heating graphene in NH3 at high temperature (≥800 °C) can
Electrical annealing, which produces
high temperature, has also been applied to obtain N-GNRs.31
The nitrogen content in the N-graphene synthesized by this
method is relatively low. Guo et al.59
obtained N-graphene with
1.1 at. % doping level at 1100 °C; Geng et al.60
the highest nitrogen content was 2.8 at. % at 800 and 900 °C.
The low doping level may be attributed to two reasons: one is
the insuﬃcient defect number in the high quality graphene, and
the other is the high annealing temperature, which will break
the C−N bonds in N-graphene.61
Moreover, the nitrogen
doping is more likely to occur at the defects and edge of
graphene in the thermal treatment method. Geng et al.60
Figure 2. Schematic illustration of the segregation technique for growing N-doped graphene.50
Figure 3. Schematic illustration for N-graphene synthesized from the
reaction of CCl4 and Li3N.52
ACS Catalysis Review
dx.doi.org/10.1021/cs200652y | ACS Catal. 2012, 2, 781−794783
pyridinic and pyrrolic N dominated in the N-graphene. Wang
claimed that nitrogen atoms preferred functionalizing
the edge of GNRs. Interestingly, unlike NH3, annealing N+
irradiated graphene in N2 at high temperature cannot introduce
nitrogen into the graphene,59
which suggests that the inertness
of N2 makes it diﬃcult to react with the reactive carbon atoms
on the defect sites in graphene.
Apart from graphene, graphene oxide can also be used to
synthesize N-graphene by thermal treatment in the presence of
various nitrogen precursors. Sheng et al.62
annealing GO in the presence of melamine at high temperature
(700−1000 °C) could produce N-graphene. The layer
distribution of N-graphene depends on the synthesis procedure.
Few-layer N-graphene is obtained if annealing the mixture of
GO and melamine at high temperature, and single layer N-
graphene can be produced if heating single-layer GO covered
with melamine. The nitrogen content is aﬀected by both the
temperature and the mass ratio between GO and melamine.
The largest nitrogen content (10.1 at. %) is obtained under 700
°C when the mass ratio of GO to melamine is 0.2. Li et al.63
showed that placing GO in an NH3 atmosphere through
thermal annealing (500 °C) could reduce GO and get N-
graphene with a 5 at. % nitrogen doping level. Notably, both of
these works report that the temperature has the major inﬂuence
on the nitrogen content of N-graphene. Li et al.63
reason to the decreased content of oxygen functional groups at
higher temperature. Because these oxygen functional groups are
responsible for the formation of a C−N bond, the reactivity
between GO and nitrogen atoms will decrease after these
groups decompose at higher temperature, resulting in the lower
nitrogen content. Moreover, it has been claimed that lowering
the mass ratio between GO and melamine at 800 °C induced
higher nitrogen doping level, which may suggest the
competitive doping between oxygen and melamine.62
2.2.2. Plasma Treatment. When carbon material is placed in
the nitrogen plasma atmosphere, carbon atoms will be partly
replaced by nitrogen atoms; therefore, this method was applied
to synthesize N-CNTs.64−66
Recently, it has been reported that
N-graphene could be prepared from graphene23,67,68
by exposing it to the nitrogen plasma. NH3 plasma has also
been used to obtain N-graphene from mechanically exfoliated
The nitrogen content, which can be controlled by
the plasma strength and exposure time, varies from 3 to 8.5 at.
% in diﬀerent works. During the plasma exposure process,
defects and oxygen-containing groups are created.23,68
showed that graphene contains 3.5 at. % oxygen species
while the N-graphene contains 8.6 at. % oxygen species, Wang
reported that the content of oxygen species increased
from about 15 to 26−28 at. % after doping. These results
indicate the plasma treatment introduces a signiﬁcant amount
of oxygen species into graphene. The reason may be ascribed to
the reactive carbon atoms at the edge of defects that are created
by the plasma treatment.23
Notably, in the N2 plasma
treatment, overexposure may decrease the electrocatalytic
activity of N-graphene.68
It has been reported that if graphene
was exposed to the N2 plasma over 40 min, the reduction
current of H2O2 would decrease because of the destruction and
split of the graphene plane.
2.2.3. Hydrazine Hydrate (N2H4) Treatment. Using
hydrazine hydrate to prepare graphene from GO is a widely
used method. Recently, N-graphene has been obtained by
reducing GO in the NH3 and N2H4 mixed solution.71
nitrogen content reaches up to 5 at. % when the reduction
temperature is 80 °C; however, the absorbed N2H4 takes a non-
negligible proportion in the total nitrogen content. If the
reaction temperature rises to 160 °C or higher, the N2H4 will
be desorbed and the nitrogen content decreases to ∼4 at. %.
Interestingly, the morphology of N-graphene also changes with
the temperature. The relative ﬂat N-graphene is generated if
GO is reduced at low temperature (≤120 °C), whereas the
obvious agglomeration in N-graphene will occur if the
temperature is higher.
By using ultrasonication,72
N-graphene can be synthesized
from graphene in the presence of N2H4. The agglomerated
regions are also observed after doping. The nitrogen content is
around 1 at. %. In addition to these, the nitrogen species in the
N-graphene contains only pyridinic and pyrrolic nitrogen. The
content and bonding conﬁguration of nitrogen indicates the
nitrogen atoms can be introduced only to the graphene edges
and defects in this method.
3. CHARACTERIZATION TECHNIQUES FOR STUDYING
3.1. X-ray Photoelectron Spectroscopy (XPS) Techni-
que. XPS is the standard technique to study the nitrogen-
doping eﬀect in graphene. In the XPS spectrum of N-graphene,
the peaks appearing at about 400 and 284 eV correspond to the
N1s and C1s, respectively. The ratio of peak intensity between
N1s and C1s is used to determine the nitrogen content in N-
graphene. Moreover, the N1s spectrum is used to determine
the nitrogen conﬁgurations. In the research about N-graphene,
the N1s spectrum usually can be deconvoluted to several
individual peaks that are assigned to pyridinic N (398.1−399.3
eV), pyrrolic N (399.8−401.2 eV), and quaternary N (401.1−
402.7 eV) (Figure 4). The peak position of these nitrogen types
varies in a relatively wide range in diﬀerent studies. Reddy et
reported the pyrrolic N appeared at 401.2 eV, whereas Li
showed the quaternary N appeared at about 401.1 eV.
The large diﬀerence of the peak positions of nitrogen
conﬁgurations may be due to the diﬀerent environments of
The charge of nitrogen and its neighbor atoms and
the electron redistribution after ionization will all inﬂuence the
precise position of diﬀerent nitrogen types. Apart from these
three nitrogen types, peak corresponding to N-oxides of
pyridinic N is observed at ∼402.8 eV in several studies.23,62
When nitrogen atoms are doped into graphene, peaks at the
C1s spectrum will change accordingly.50,62,63,70,71
In the C1s
spectrum of GO (Figure 5a), the sharp peak at around 284.5 eV
corresponds to the sp2
carbon with CC bonds. Another
strong peak at higher energy corresponds to the sp3
Figure 4. High-resolution N1s XPS spectra of graphene and N-
graphene. N1 represents pyridinic N, N2 represents pyrrolic N, N3
represents quaternary N, and N4 represents the N oxides of pyridinic
ACS Catalysis Review
dx.doi.org/10.1021/cs200652y | ACS Catal. 2012, 2, 781−794784
with several diﬀerent C−O bonding conﬁgurations. These
conﬁgurations include the C−O bonds, carbonyls (CO), and
carboxylates (OC−O) at about 286.2, 287.8, and 289.2 eV,
respectively. After GO is annealed in Ar, the intensity of the
peak ascribed to the C−O bonding conﬁgurations decreases to
a much lower value (Figure 5b).62
This indicates that most of
the oxygen groups in GO are removed after annealing. If GO is
doped with nitrogen atoms (Figure 5c), peaks ascribed to C−O
bonding conﬁgurations disappear, and new small peaks appear
after peak ﬁtting.50,62,70,71
In the work of Sheng et al.,62
peaks appearing at 285.8 and 287.5 eV were assigned to the sp2
carbon atoms, respectively. In other works,50,70
small peak at ∼289 eV was observed. This peak is ascribed to
the physisorbed oxygen on the graphene. Generally speaking,
the peak change at higher energy in the C1s spectrum suggests
the nitrogen doping occurs in the graphene.
3.2. Raman Spectroscopy. Raman spectroscopy is another
very useful method to characterize N-graphene. The D, G, and
2D bands are the predominant features in the spectrum of N-
graphene. They are represented by peaks at around 1320−
1350, 1570−1585, and 2640−2680 cm−1
, respectively (Figure
6.) In some studies,40,52
the peak called D′ will appear at
. These bands already have been studied
intensively in former studies.74−78
Speciﬁcally, the G band
corresponds to the doubly degenerate E2g phonons at the
Brillouin zone. It originates from the ﬁrst-order Raman
scattering process. The 2D and D bands are all induced by
the second-order, double-resonance process and related to
zone-boundary phonons. The scattering process involves two
zone-boundary phonons for 2D mode; it involves one phonon
and one defect for the D mode. Diﬀerent from the D band
which requires defects to activate it, the 2D band does not
require the activation of defects. Thus, the 2D band is always
seen in the Raman spectra of graphene and N-graphene, even
when the D band cannot be observed. For the D′ band, it arises
from the intravalley, defect-induced, double-resonance process.
have revealed that the intensity ratio of
the D and G bands (ID/IG) was inversely proportional to the in-
plane crystallite sizes La. The crystallite size can be determined
according to the Tuinstra−Koenig (TK) relation, La(nm) =
(2.4 × 10−10
(λ is the Raman excitation
wavelength). For nitrogen doping, the substitution of nitrogen
atoms usually is accompanied by the introduction of defects
into the graphene surface. Considering La as the average
interdefect distance, more defects undoubtedly means a smaller
La; thus, La can be used to study defects introduced by nitrogen
doping. Comparing the crystallite size of pristine graphene with
N-graphene, Zhang et al.50
reported that the ID/IG of graphene
and N-graphene with lower (NG1) and higher (NG2) nitrogen
doping level are 0.26, 0.8 and 2.1, which corresponds to
crystallite sizes of 65, 21, and 8 nm, respectively (Figure 7).
This suggests the crystallite size decreases remarkably with an
increase in the nitrogen doping level because of the defects.
Apart from ID/IG, the intensity ratio of the 2D and G bands
(I2D/IG) has been used to characterize N-graphene. It has been
reported that I2D/IG depends on the electron concentration
The G band always stiﬀens, and the 2D band
responds diﬀerently to hole and electron doping; thus, I2D/IG
has been used to estimate the nitrogen doping level.50,70
Through calculating the I2D/IG, which was <0.6 in N-graphene,
it was concluded that the doping level was higher than 4 × 1013
Notably, some studies also presented that the G band
increased almost linearly, corresponding to the increment of
Figure 5. High-resolution C1 spectra of the (a) GO, (b) graphene prepared by annealing GO in Ar at 800 °C, and (c) N-graphene prepared by
annealing GO/melamine (1:5) at 800 °C for 30 min.62
Figure 6. Typical Raman spectrum of N-graphene transferred onto a
SiO2/Si substrate. The laser excitation wavelength is 514.5 nm.44
Figure 7. Raman spectra of pristine graphene and N-graphene with 0.6
(NG1) and 2.9 (NG2) at. % doping level. The insert shows the
enlarged 2D band of NG2. The laser excitation wavelength is 514.5
ACS Catalysis Review
dx.doi.org/10.1021/cs200652y | ACS Catal. 2012, 2, 781−794785
and IG/I2D was related to the thickness of the
Thus, for N-graphene with inhomogeneous
layers, the I2D/IG cannot reﬂect the nitrogen doping level.
I2D/IG can be used only when N-graphene has homogeneous
Before using ID/IG and I2D/IG to characterize N-graphene,
inhomogeneous nitrogen doping should be considered. It has
been reported that some spots showed high ID/IG and some
showed very low ID/IG within the N-graphene,40
the nonuniform defect distribution induced by inhomogeneous
nitrogen incorporation. Thus, the ID/IG and I2D/IG derived
from the Raman spectra at discrete spots cannot fully reﬂect the
doping situation. In practice, Raman spectral mapping can be
used to avoid this problem. This technique records the Raman
spectra on a large scale; thus, the comparison of diﬀerent N-
graphenes is more convincing for inhomogeneous doping. In
the maps of I2D/IG over a 80 × 80 μm2
area (Figure 9b),84
pristine graphene shows a higher I2D/IG, which means a lower
carrier concentration. The more area of low I2D/IG in N-
graphene grown under higher NH3 ratio corresponds to a
higher carrier concentration. Moreover, it is observed that the
size of the purple paths depends on the doping level, which
indicates the purple paths are related to the local dopant
Some studies reported a shift of the G band after nitrogen
doping. Because the variation of charge density in pristine
graphene will cause the diﬀerent G band positions and I2D/IG in
the diﬀerent spots of graphene,85
Li et al. made a gold marker
in the vicinity of graphene to accurately monitor the evolution
of the nitrogen doping.70
An upshift of the G band in the
Raman spectra of the monolayer graphene was observed. In the
work of Zhao et al.,84
a similar trend of the G band was also
observed by using the frequency histogram collected from
Raman spectral mapping (Figure 9d). However, the observed
position of the G band can also be aﬀected by the
inhomogeneous layer distribution82,86
and defects due to
which may induce the downshift of G
band in N-graphene in some studies.52,63
consideration should be taken if discussing this phenomenon.
3.3. Scanning Tunneling Microscopy (STM). STM is a
very powerful technique to investigate the electronic properties
of a sample. It can probe the charge density at the Fermi level.
When the bias voltage (Vbias) applied between the tip and
sample is positive, electrons tunnel from the tip into the
specimen, then the lowest unoccupied states of the specimen
are probed. When a negative Vbias is applied, electrons tunnel
from the specimen into the tip, and the highest occupied states
of specimen are probed.88
Due to the sharp tip, the STM
images can show atomic resolution. Recently, both theoretical
and experimental studies on the electronic properties of N-
graphene have been carried out.52,84,89
Compared with the pristine graphene, N-graphene shows
some brighter sections that are distinct from the main graphene
network in the STM image (Figure 10c).52,84
features correspond to diﬀerent nitrogen doping types. Because
these bright sections are only a few atoms across (<1 nm), they
cannot be defects induced by nitrogen doping.52
STM line scan over the bright section and graphene lattice
(Figure 10a), an out-of-plane height of 0.6 ± 0.2 Å is observed.
This indicates the substitution of nitrogen atoms in graphene.
The calculated STM image shows that the C atoms neighboring
Figure 8. The inﬂuence of hole and electron doping on the I2D/IG.80
Figure 9. (a) Raman spectra taken at diﬀerent positions over N-graphene grown under 0.1 Torr NH3 (NG10). (b) Maps of I2D/IG for pristine
graphene, NG10, and N-graphene grown under 0.13 Torr NH3 (NG13). (c) Maps of the G band frequency for PG, NG10, and NG13 samples. (d)
G band frequency histogram of PG, NG10, and NG13 from the maps in part c.84
ACS Catalysis Review
dx.doi.org/10.1021/cs200652y | ACS Catal. 2012, 2, 781−794786
N atoms exhibit the brightest feature because of the increased
charge density of state induced by the neighbor N atoms
Apart from the local structure around dopants, some long
“tails” arising from the intervalley electron scattering are
observed in the STM image (Figure 10c). This kind of
scattering is veriﬁed by the inner hexagon in the fast Fourier
transform (FFT). STM is also used to study the possibility of
dopant clustering. The dopant distribution in the N−N
distance is quadratic even when the distance is down to few
lattice constants (Figure 10d); it indicates that the dopants
distribute randomly. Furthermore, the study reveals that nearby
dopants prefer to substitute into the same sublattice of
graphene. The charge-carrier density of N-graphene can be
measured from a STM study. From the curves of dI/dV
(derivative of current with respect to the voltage), the Dirac
point of N-graphene is calculated (Figure 10e). Then the
charge-carrier density can be calculated from the relation n =
(n is the charge-carrier density, h̅ is the Plank’s
constant over 2π, νF is the Fermi velocity).
3.4. Other Characterization Techniques. In addition to
the above techniques, scanning electron microscope (SEM),
HRTEM, atomic force microscope (AFM), selected area
electron diﬀraction (SAED) and thermogravimetric analysis
(TGA) have also been used to study N-graphene. Speciﬁcally,
SEM is commonly employed to study the morphology of N-
graphene. HRTEM is the most commonly used technique to
determine the number of graphene layers on the basis of the
cross section or edge images of N-graphene. AFM can also be
used to estimate the number of graphene layers on the basis of
the interlayer distance. SAED can provide information about
the crystalline structure of N-graphene on the basis of
diﬀraction pattern. The hexagonal diﬀraction spots indicate
that the N-graphene still keeps a well-ordered crystalline
and the ringlike diﬀraction pattern of spots
means structure distortion occurs after doping.41
4.1. Electrocatalyst for Fuel Cell Application. A fuel cell
is an electrochemical energy conversion device that oxidizes
fuel at the anode and reduces oxygen from air at the cathode to
Commonly, Pt is used as the catalyst for
the oxidation reaction on the anode and reduction reaction on
cathode. However, the commercial application of Pt catalysts is
limited by its scarcity, time-dependent drift, and CO poison-
Thus, Pt-based catalysts91,92
and other metal catalysts,
such as Au and Pd,93,94
have been developed. Recently, N-
graphene has been used in fuel cells as either the catalysts
directly or carbon support to anchor metal catalysts.
4.1.1. Theoretical Part. The oxygen reduction reaction of N-
graphene on the cathode of a fuel cell has been discussed in
many studies. Through studying the ORR behavior of model
graphenes C45NH20 and C45NH18 in acidic environment, Zhang
showed that the spin density and charge density of
atoms were the major factors that determined the catalytic
active sites in ORR. The substitution of N atoms, which
introduces the unpaired electron, will change the atomic charge
distribution. The active sites in N-graphene usually are carbon
atoms that possess high spin density. If the spin density is
negative and small, the atom with a higher charge density will
be the active sites. Although in a previous study,95
it was shown
that the energy gap between highest occupied molecular orbital
(HOMO) and lowest unoccupied molecular orbital (LUMO)
could be used as an index of kinetic stability, it is unnecessarily
related to the catalytic capacity of graphene and N-graphene.
The ORR mechanism on N-graphene also has been studied.
Earlier studies have shown that O2 could be reduced following
two pathways. One is a direct four-electron pathway in which
O2 is reduced to water in an acidic environment or OH−
alkaline environment. Another is a two-electron pathway in
which O2 is partly reduced to H2O2 in an acidic environment or
in an alkaline environment. Both mechanisms have
been proposed by theoretical studies based on diﬀerent N-
graphene models. Kurak et al.96
showed a two-electron ORR
pathway based on the graphene model possessing two neighbor
Figure 10. (a) STM image of the most common doping form in N-graphene. The inset is the line proﬁle across the dopant (Vbias = 0.8 V, Iset = 0.8
nA). (b) Simulated STM image of quaternary N dopant based on density functional theory calculations (Vbias = 0.5 V). (c) STM image of N-
graphene showing ∼14 quaternary N dopants. The inset is the FFT of topography (Vbias = 0.8 V, Iset = 0.8 nA). (d) Spatial distribution of N−N
distances from eight samples with diﬀerent nitrogen concentrations. (e) dI/dV curves taken from an N atom and other nearby bright topographic
features (Vbias = 0.8 V, Iset = 1.0 nA).84
ACS Catalysis Review
dx.doi.org/10.1021/cs200652y | ACS Catal. 2012, 2, 781−794787
N atoms in the zigzag edge. However, it was found that two
nitrogen atoms were very unlikely to be doped at two
neighboring zigzag sites by checking the interaction energy
between two nitrogen atoms.97
Zhang et al.25
proposed a four-electron ORR pathway on N-
graphene in an acidic environment. Furthermore, after taking
the solvent, surface coverage, and adsorbates into consideration,
Yu et al.98
obtained the overall energy proﬁle of the ORR
pathway on N-graphene in an alkaline environment. The study
shows that water molecules are essential for the reaction. The
O2 adsorption is greatly enhanced due to the O2 polarization
induced by the hydrogen bonding with water. Through
investigating two ORR mechanisms, dissociative and associative
(Figure 11), study shows that the associative mechanism is
more energetically favored in ORR because of the lower O2
dissociation barrier. In the associative mechanism, the
desorption barrier of OOH(ads) into OOH−
is high, so the
energetically favored reaction OOH(ads) → O(ads) + OH−
more likely to happen, which suggests the four-electron ORR
pathway of N-graphene. The reaction rate is determined by the
removal of O(ads) on the surface of N-graphene.
Apart from N-graphene, the interaction between Pt atom and
N-graphene has been investigated.26
In N-graphene, the
nitrogen atoms do not bond with Pt atom directly; instead,
they direct a Pt atom to bond with the carbon atom, which is
more energetically favored. This is helpful to prevent Pt
nanoclusters from migrating and forming larger particles.
Because the introduction of nitrogen atoms disrupts the
delocalized double bond in the graphene system, the Pt/C
bond will focus on the 6s/2s orbitals rather than 5d/2p orbitals.
This doubles the binding energy between Pt and carbon atoms.
In general, the binding of Pt to N-graphene improves the
catalytic durability of Pt.
4.1.2. Experimental Part. Several groups have recently
reported studies on metal-free N-graphene with enhanced
catalytic activity toward ORR.23,40,41,52,60,62
The eﬃciency of
ORR can be evaluated through two ways.99
One way is to
calculate the transfer number of electrons through the
Koutecky−Levich (K−L) equation by using a rotating disk
electrode (RDE). Another way is to measure the proportion of
H2O2 formed during the ORR process by using a rotating ring-
disk electrode. Qu et al.41
reported that N-graphene exhibited a
typical one-step, four-electron ORR pathway, which is similar
to the ORR pathway of a Pt catalyst (Figure 12a). In contrast,
pristine graphene showed a two-step, two-electron ORR
pathway with a lower onset potential. In another work,60
H2O2 formed in the ORR process was about 10% at −0.5 V in
the diﬀusion-controlled region. The low proportion of H2O2
indicated the four electron reduction process dominated in
ORR. All these studies show that N-graphene can be a very
eﬀective catalyst for ORR.
Furthermore, the ORR activity of N-graphene is also studied
through diﬀusion limited current and kinetic current. Some
studies showed the diﬀusion-limited current density of N-
graphene was higher than commercial 20% or 40% Pt/C (E-
but another study showed that N-graphene
had a similar diﬀusion-limited current density.60
reported activity of N-graphene varies from diﬀerent studies,
there is consensus that N-graphene has excellent stability
compared with the Pt catalyst. Shao et al.23
reported that the
20% Pt/C (E-TEK) showed higher electrocatalytic activity than
N-graphene before an accelerated degradation test (ADT), but
after the ADT, the N-graphene exhibited higher kinetic current
compared with the Pt/C catalyst because of the degradation of
Pt/C. In addition, studies also showed the activity of N-
graphene would not be inﬂuenced by the addition of methanol
or CO (Figure 12b).23,41
These two advantages make N-
graphene a promising material toward ORR in fuel cells.
Notably, in the above studies in which the four-electron ORR
pathway was observed, these N-graphene catalysts consist of
two or three nitrogen types.23,41,52,60,62
possessing only the pyridinic N, a two-electron reduction
process was observed in the ORR process.40
This may indicate
a less eﬃcient ORR performance of pyridinic N. In another
study, the N-graphene with higher pyridinic and quaternary N
content exhibited a higher onset potential than N-graphene that
possessed the same nitrogen content. This suggests the
pyridinic and quaternary N may play a more important role
for ORR activity.60
However, because of the scarcity of study in
this ﬁeld and variation in experimental conditions, the
relationship between the catalytic activity and the nitrogen
species is still unclear. In the former study of N-CNTs, both
nitrogen have been
observed to have the dominant eﬀect for the ORR activity.
Thus, further research work on the nitrogen catalytic site is still
Figure 11. Scheme of the ORR reaction on N-graphene in an alkaline
environment where 1 is the associative mechanism and 2 is the
Figure 12. (a) RRDE voltammograms for ORR in air-saturated 0.1 M
KOH on the electrodes graphene (red), Pt/C (green), and N-
graphene (blue) with a scan rate of 0.01 V s−1
. Electrode rotating rate:
1000 rpm. (b) Current−time chronoamperometric response of Pt/C
and NG to CO. The arrow indicates the addition of 10% (v/v) CO at
ACS Catalysis Review
dx.doi.org/10.1021/cs200652y | ACS Catal. 2012, 2, 781−794788
Apart from the nitrogen types, the nitrogen content is also
related to the ORR activity of N-graphene. However, because
N-graphene usually consists of two or three nitrogen types and
the content of diﬀerent nitrogen types usually varies with
diﬀerent nitrogen doping levels, diﬀerent studies have produced
contradictory results in previous studies.52,62
In a more direct
study in which N-graphene contains only pyridinic N,40
graphene possessing the higher nitrogen content (16 at. %)
exhibited poorer ORR activity than that possessing the lower
nitrogen content (2.2 at. %). In a theoretical study, it has been
reported that model graphene with a higher nitrogen content
was more easily poisoned by O(ads) because of the stronger
These results mean an optimal nitrogen content
might be critical to achieving a high ORR activity.
Several studies also have studied the performance of Pt/N-
graphene in both oxidation and reduction reactions.67,73
Pt/N-graphene used for an oxidation reaction,73
it has been
reported that Pt nanoparticles could disperse better on the
surface of N-graphene with the existence of N atoms in a
carbon lattice. Moreover, the conductivity of N-graphene was
improved at high temperature (800 °C). These two factors
made Pt/N-graphene exhibit a 3 times higher oxidation current
than 20% Pt/carbon black catalyst. For Pt/N-graphene used for
the oxygen reduction reaction,67
it also showed an improved
performance compared with Pt/graphene because of the better
dispersion of Pt nanoparticles and stronger interaction between
Pt and C atoms stated in the theoretical part.26
Apart from the Pt catalyst, other nonprecious metal catalysts
supported on N-graphene toward ORR have been stud-
Tsai et al.103
synthesized FeCN/N-graphene by
impregnating N-graphene into a mixture of iron acetate and
1,10-phenanthroline, then the FexC species formed in the
sintering process would anchor the FeCN nanoparticles on N-
graphene surface. The as-synthesized FeCN/N-graphene shows
an enhanced ORR activity compared with the N-graphene
because of the additional ORR activity of FeCN nanoparticles.
In another notable study,104
Liang et al. grew Co3O4 on mildly
oxidized graphene oxide (rmGO) with or without the presence
of NH4OH, then catalyst Co3O4/rmGO and Co3O4/N-rmGO
were obtained. The latter catalyst has ∼4 at. % nitrogen
content. Through the ORR study of the Co3O4/rmGO and
Co3O4/N-rmGO, it has been revealed that these two catalysts
exhibit high ORR activity that is diﬀerent from the Co3O4
nanocrystals (Figure 13a). Also diﬀerent from the two-electron
ORR pathway of N-rmGO obtained in the study, these two
catalysts show the obvious four-electron ORR pathway (Figure
13b, c). Comparing the kinetic current of Co3O4/N-rmGO
with Co3O4/rmGO, the former exhibits the apparent higher
current density than the latter (Figure 13d). The higher ORR
activity of Co3O4/N-rmGO is ascribed to the synergistic
coupling between Co3O4 and N-graphene. Because Co3O4/N-
rmGO shows both the high ORR activity similar to Pt catalyst
and excellent stability, this kind of hybrid catalyst is also
promising for ORR catalysis.
4.2. Field-Eﬀect Transistor (FET). For semiconductors,
the ﬂow of electricity needs some kind of activation (for
example, heat or light absorption) to get over the gap between
the valence band and conduction band.105
If the semiconductor
is activated by the external electric ﬁeld to switch “on” and “oﬀ”,
then it is called FET. Generally speaking, the large-scale and
Figure 13. (a) Cyclic voltammetry (CV) of Co3O4/rmGO, Co3O4/N-rmGO and Pt/C in O2- (solid line) or Ar-saturated (dashed line) 0.1 M KOH
solution. RDE voltammograms of Co3O4/rmGO (b) and Co3O4/N-rmGO (c) for ORR in O2-saturated 0.1 M KOH at diﬀerent rotation rates with a
scan rate of 5 mV s−1
. The inset ﬁgure is the corresponding Koutecky−Levich plots at diﬀerent potentials. (d) Tafel plots of Co3O4/rmGO and
Co3O4/N-rmGO derived by the mass-transport correction.104
ACS Catalysis Review
dx.doi.org/10.1021/cs200652y | ACS Catal. 2012, 2, 781−794789
bilayer graphene do not possess a band gap; however,
constraining large-scale graphene in one dimension (GNRs)
or applying an electric ﬁeld perpendicularly on the bilayer
graphene can induce the band gap (Figure 14).106
both theoretical and experimental works have studied the
semiconductor properties of N-graphene.
4.2.1. Theoretical Part. Nitrogen doping can eﬀectively
modulate the electrical properties of graphene. On the basis of
the investigation of C3N4 and C6N9H3 graphene,29
it has been
revealed that the band gap of N-graphene with a high N/C
ratio reached ∼5 eV. The band gap can be tuned by the
presence of external stress or adatoms. In another theoretical
work based on the study of delta-doping graphene,107
been reported that the band gap could be opened only when
the nitrogen content was over ∼25%. However, delta-doping
may be unlikely to occur in practice. In the experimental study,
an obvious band gap has been observed on N-graphene with a
lower nitrogen content.70
Apart from the band gap, the
mobility and conductivity of N-graphene has also been
discussed theoretically by using the quantum-mechanical
When the nitrogen concen-
tration (Cd) is over or equal to 2% (2% ≤ Cd ≤ 4%), the decay
of the diﬀusion coeﬃcient D is clearly observed. This indicates
the onset of quantum interference eﬀects. However, this eﬀect
is still weak and can only marginally aﬀect the conduction when
the nitrogen content is low. This study suggests that the
nitrogen doping may modulate the graphene property while
maintaining good mobility and conductivity. However, the
conduction is also inﬂuenced by many other factors. In
experimental study, it has been shown that both defects and
nitrogen atoms will be introduced into graphene. Defects can
serve as the scattering center, which will aﬀect the mobility of
N-graphene. Moreover, when the nitrogen concentration rises
over 5%, a stronger localization eﬀect might occur, which will
largely decrease the mobility in N-graphene.27
GNR can be obtained by constraining large-scale graphene to
one dimension. Former studies have revealed that H-
terminated GNRs with either armchair or zigzag-shaped
edges have nonzero band gaps.7,9,108
studies of zigzag GNR (ZGNR),109,110
it was revealed that the
nitrogen atom and defects energetically preferred to dope at the
edge of GNR. Depending on doping sites and various GNRs,
the introduction of nitrogen atoms will induce very diﬀerent
electronic properties. For example, Yu et al.109
nitrogen doping sites would make the impurity state lie below
or above the Fermi level. Li et al.110
found one edge-doped
nitrogen made ZGNR spin a gapless semiconductor while two
opposite edge-doped nitrogens made ZGNR nonmagnetic
metals. Biel et al.111
reported that the full suppression of
impurity backscattering would occur if the doped GNR was
armchair and mirror-symmetrical.
4.2.2. Experimental Part. After the preparation of bottom-
gated N-graphene FET by using a Si substrate with a 500 nm
thick SiO2 layer (Figure 15a), pristine graphene exhibits p-type
behavior because of the adsorption of oxygen or water in air
(Figure 15b). In contrast, N-graphene with a 8.9 at. % nitrogen
Figure 14. Band structure around the k point of (i) large-area
graphene, (ii) graphene nanoribbons, (iii) unbiased bilayer graphene,
and (iv) bilayer graphene with an applied perpendicular ﬁeld.106
Figure 15. (a) Schematic illustration of the N-graphene FET device. (b, c) Ids/Vds characteristics at various Vg's for the pristine graphene and NG
FET device. (d) Transfer characteristics of the pristine graphene and the NG.30
ACS Catalysis Review
dx.doi.org/10.1021/cs200652y | ACS Catal. 2012, 2, 781−794790
doping level exhibits typical n-type semiconductor behavior
(Figure 15c, d).30
Compared with the mobility of pristine
graphene (300−1200 cm2
), the mobility of N-graphene
reduces to 200−450 cm2
. Using diﬀerent precursors in
the CVD method, Jin et al.44
reported the mobility of N-
graphene with 2.4 at. % nitrogen content reduced by 2 orders of
magnitude compared with that of pristine graphene. In other
such as N-graphene obtained through NH3
annealing after N+
a much lower hole and
electron conductivity was observed compared with the pristine
In the study of nitrogen-doped GNR (N-GNR), it has been
reported the N-GNR fabricated by high power electrical
annealing in NH3 showed typical n-type semiconductor
behavior, and the mobility was similar with the GNR annealed
The reason is that nitrogen atoms incorporate
mainly into the edge of GNR, and few charged impurities are
introduced, which will not degrade the mobility of GNR.
As discussed above, the electron mobility of graphene
decreases with the increment of band gap in most cases, which
is similar to the trend in studies of CNTs.106,112,113
several theoretical studies27,111
and the recent work about N-
have shown the mobility of N-graphene might be
maintained by controlling the nitrogen at a low doping level
and speciﬁc doping site, the scattering center induced by the
defects will drastically decrease the mobility of N-graphene in
practice. In addition, it is claimed that the grain boundaries in
N-graphene may also contribute to a decrement of mobility.36
Other than the mobility, a sizable band gap, preferably 0.4 eV
or higher, is also required in conventional FET (the band gap of
silicon is 1.1 eV).106
Until now, only a few studies of N-
graphene have reported a band gap in their works. Zhang et al.
showed the band gap in N-graphene with 2.9 at. % nitrogen
content was about 0.16 eV,50
which is still too low. Considering
the mobility and band gap of N-graphene obtained up to the
present, synthesization of N-graphene for practical applications
is still far oﬀ.
4.3. Lithium Ion Batteries. In recently years, graphene has
attracted great attention as a potential anode material in lithium
ion batteries (LIBs) because of its fascinating properties, such
as high electrical electronic properties, high surface area, and
excellent mechanical ﬂexibility. Although graphene-based
materials can reach a high reversible capacity (1013−1054
mA h/g) at a low charge rate,114
it is still rate-limited at a high
charge/discharge rate (≥500 mA/g).115
Thus, a N-graphene-
based device is proposed with the intent to achieve a high
reversible capacity at the high charge/discharge rate.
In earlier work, Reddy et al.43
obtained N-doped graphene
under the control of a CVD method. The reversible discharge
capacity of N-graphene was almost double compared with
pristine graphene because of the enhanced Li ion intercalation
with the introduction of nitrogen atoms. In another more
N-GNS with 2 at. % nitrogen content (57.4%
pyridinic, 35.0% pyrrolic, and 7.6% quaternary N) was
synthesized by heat treatment of GO in an NH3 atmosphere.
The N-graphene possessed a reversible capacity of around 900
mA h/g at a current density of 42 mA/g and a capacity of ∼250
mA h g−1
at a high current density of 2.1 A/g. In another work
in which N-graphene was synthesized by a similar heat
N-graphene with 3.13 at. % nitrogen
content exhibited reversible capacities of 1043 mAh/g and 872
mAh/g in the ﬁrst and 31st cycles at a low current rate of 50
Figure 16. Galvanostatic charge−discharge proﬁle of N-graphene at a low current rate of 50 mA/g (a) and a higher current rate from 0.5 to 25 A/g
(c), (b) cycle performance and Coulombic eﬃciency of N-graphene at low current rate of 50 mA/g, (d) cycle performance and rate capabilities of N-
graphene at higher current rate from 0.5 to 25 A/g.115
ACS Catalysis Review
dx.doi.org/10.1021/cs200652y | ACS Catal. 2012, 2, 781−794791
mA/g, respectively (Figure 16 a, b). At a higher current rate of
25 A/g, the reversible capacities of N-graphene still reached 199
mAh/g (Figure 16 c, d).
The excellent performance of N-graphene can be ascribed to
many factors, such as the introduction of nitrogen atoms, the
defects and disordered surface morphology induced by doping,
increased electrode/electrolyte wettability, and improved
electrochemical performance. Notably, in the above studies,
the types of pyridinic and pyrrolic N are predominant in the N-
graphene. Through the study of nitrogen-doped graphite, it has
been revealed that both the pyridinic and quaternary N played
an eﬀective role in lithium intercalation and extraction.117
graphene with a large quaternary N content might also be used
4.4. Devices in Other Fields. N-Graphene has been
applied in the ﬁeld of ultracapacitors.69
based on N-graphene has shown a long cycle life (Figure 17a).
Moreover, a N-graphene-based device showed a much higher
capacitance than a device based on pristine graphene in both
KOH and organic electrolyte (Figure 17b). By calculating the
binding energy between the potassium ion and nitrogen
conﬁgurations at diﬀerent positions of N-graphene, it has been
revealed that the basal-plane pyridinic N exhibited the largest
binding energy. Thus, basal-plane pyridinic N was claimed to
have a dominant role in the capacitance enhancement. Pyrrolic
N also showed a large binding energy with ion, but the negative
charge of pyrrolic N would cause too strong binding for the
reversible charging/discharging process, which was reﬂected by
the lower Coulombic eﬃciencies of N-graphene with a large
proportion of pyrrolic N. Therefore, controlling the appropriate
nitrogen conﬁguration can greatly promote the capacitance of
Study has shown that N-graphene has a better electron
transfer eﬃciency than pristine graphene,68,72
potential use for electrochemical sensing. Because glucose
oxidase (GOx) could oxidize glucose with oxygen and produce
gluconic acid and H2O2, Wang et al.68
fabricated the glucose
sensor by immobilizing GOx on the biocompatible N-graphene
surface. It was observed that the GOx redox peak current on N-
doped graphene was greatly improved over that on graphene,
which demonstrated the enhanced electron transfer eﬃciency
of N-graphene. This kind of biosensor shows a good response
for glucose concentrations ranging from 0.01 to 0.5 mM in the
presence of other molecules.
Apart from the above applications, N-graphene also has been
used as a support to anchor quantum dots toward high-
sites have a higher photocatalytic activity than graphene/CdS
and pure CdS, which can be attributed to the hampering of the
radiative recombination of the electron−hole pairs induced by
enhanced electron transportation from CdS to N-graphene.
Moreover, CdS anchored on N-graphene with 2 wt % nitrogen
content showed the best catalytic activity. It reveals that a
proper junction structure is required for the highest photo-
In summary, many research works on N-graphene have
emerged in recent years. Various synthesis approaches and
characterization techniques have been explored to obtain and
characterize N-graphene. The N doping oﬀers an eﬀective way
to tailor the properties of graphene, thus making N-graphene a
promising material for use in many ﬁelds. However, the method
for the production of large-scale N-graphene is still lacking;
thus, new methods are required. Moreover, synthesizing N-
graphene meets problems similar to those encountered during
fabricating N-CNT. First, controlling the nitrogen type and
distribution is unresolved. Second, to achieve nitrogen doping
at speciﬁc positions and with precise control of doping content
is still a challenge. For FET application, the doping location and
doping content is critical not to decrease the electron mobility
drastically while opening a suitable band gap. For electro-
catalysis, the correlation between the activity and nitrogen type
needs to be identiﬁed, and controlling the speciﬁc nitrogen type
in N-graphene is required for high performance catalysts. For
other applications, such as LIBs and ultracapacitors, a speciﬁc
nitrogen type may also be required. Another issue to be
considered is defects and distortion. Defects are inevitable
during the synthesis process of N-graphene. They will decrease
the mobility of N-graphene; however, their presence will
beneﬁt the catalytic reaction for ORR and LIBs. Depending on
the application, choosing or ﬁnding an appropriate approach is
■ AUTHOR INFORMATION
*Phone: (65) 6316 8866. Fax: (65) 6794 7553. E-mail:
The authors declare no competing ﬁnancial interest.
This work is supported by the academic research fund AcRF
tier 2 (MOE2009-T2-2-024), Ministry of Education, Singapore,
and competitive research program (2009 NRF-CRP 001-032),
National Research Foundation, Singapore.
(1) Novoselov, K. S.; Geim, A. K.; Morozov, S. V.; Jiang, D.; Zhang,
Y.; Dubonos, S. V.; Grigorieva, I. V.; Firsov, A. A. Science 2004, 306,
(2) Stoller, M. D.; Park, S.; Zhu, Y.; An, J.; Ruoﬀ, R. S. Nano Lett.
2008, 8, 3498.
(3) Balandin, A. A.; Ghosh, S.; Bao, W.; Calizo, I.; Teweldebrhan, D.;
Miao, F.; Lau, C. N. Nano Lett. 2008, 8, 902.
(4) Lee, C.; Wei, X.; Kysar, J. W.; Hone, J. Science 2008, 321, 385.
(5) Barone, V.; Hod, O.; Scuseria, G. E. Nano Lett. 2006, 6, 2748.
(6) Kosynkin, D. V.; Higginbotham, A. L.; Sinitskii, A.; Lomeda, J. R.;
Dimiev, A.; Price, B. K.; Tour, J. M. Nature 2009, 458, 872.
(7) Li, X.; Wang, X.; Zhang, L.; Lee, S.; Dai, H. Science 2008, 319,
Figure 17. (a) The cycling tests for the ultracapacitors based on Ni
and paper substrates up to 10 000 cycles. (b) The speciﬁc capacitances
measured in 6 M KOH and organic electrolytes.69
ACS Catalysis Review
dx.doi.org/10.1021/cs200652y | ACS Catal. 2012, 2, 781−794792
(8) Ponomarenko, L. A.; Schedin, F.; Katsnelson, M. I.; Yang, R.;
Hill, E. W.; Novoselov, K. S.; Geim, A. K. Science 2008, 320, 356.
(9) Ritter, K. A.; Lyding, J. W. Nat. Mater. 2009, 8, 235.
(10) Jiao, L.; Zhang, L.; Wang, X.; Diankov, G.; Dai, H. Nature 2009,
(11) Derycke, V.; Martel, R.; Appenzeller, J.; Avouris, P. Appl. Phys.
Lett. 2002, 80, 2773.
(12) Gong, K.; Du, F.; Xia, Z.; Durstock, M.; Dai, L. Science 2009,
(13) Wang, S. Y.; Wang, X.; Jiang, S. P. Langmuir 2008, 24, 10505.
(14) Wang, S. Y.; Yang, F.; Chen, S. L.; Jiang, S. P.; Wang, X.
Electrochem. Commun. 2010, 12, 1646.
(15) Zhou, C.; Kong, J.; Yenilmez, E.; Dai, H. Science 2000, 290,
(16) Schedin, F.; Geim, A. K.; Morozov, S. V.; Hill, E. W.; Blake, P.;
Katsnelson, M. I.; Novoselov, K. S. Nat. Mater. 2007, 6, 652.
(17) Giovannetti, G.; Khomyakov, P. A.; Brocks, G.; Karpan, V. M.;
van den Brink, J.; Kelly, P. J. Phys. Rev. Lett. 2008, 101, 026803.
(18) Chen, W.; Chen, S.; Qi, D. C.; Gao, X. Y.; Wee, A. T. S. J. Am.
Chem. Soc. 2007, 129, 10418.
(19) Ewels, C. P.; Glerup, M. J. Nanosci. Nanotechnol. 2005, 5, 1345.
(20) Casanovas, J.; Ricart, J. M.; Rubio, J.; Illas, F.; Jiménez-Mateos, J.
M. J. Am. Chem. Soc. 1996, 118, 8071.
(21) Kundu, S.; Nagaiah, T. C.; Xia, W.; Wang, Y.; Dommele, S. V.;
Bitter, J. H.; Santa, M.; Grundmeier, G.; Bron, M.; Schuhmann, W.;
Muhler, M. J. Phys. Chem. C 2009, 113, 14302.
(22) Matter, P. H.; Zhang, L.; Ozkan, U. S. J. Catal. 2006, 239, 83.
(23) Shao, Y.; Zhang, S.; Engelhard, M. H.; Li, G.; Shao, G.; Wang,
Y.; Liu, J.; Aksay, I. A.; Lin, Y. J. Mater. Chem. 2010, 20, 7491.
(24) Biddinger, E. J.; Deak, D. V.; Ozkan, U. S. Top. Catal. 2009, 52,
(25) Zhang, L. P.; Xia, Z. H. J. Phys. Chem. C 2011, 115, 11170.
(26) Groves, M. N.; Chan, A. S. W.; Malardier-Jugroot, C.; Jugroot,
M. Chem. Phys. Lett. 2009, 481, 214.
(27) Lherbier, A.; Blase, X.; Niquet, Y. M.; Triozon, F.; Roche, S.
Phys. Rev. Lett. 2008, 101, 036808.
(28) Wu, M.; Cao, C.; Jiang, J. Z. Nanotechnology 2010, 21, 505202.
(29) Deifallah, M.; McMillan, P. F.; Corà, F. J. Phys. Chem. C 2008,
(30) Wei, D.; Liu, Y.; Wang, Y.; Zhang, H.; Huang, L.; Yu, G. Nano
Lett. 2009, 9, 1752.
(31) Wang, X.; Li, X.; Zhang, L.; Yoon, Y.; Weber, P. K.; Wang, H.;
Guo, J.; Dai, H. Science 2009, 324, 768.
(32) Huang, X.; Yin, Z.; Wu, S.; Qi, X.; He, Q.; Zhang, Q.; Yan, Q;
Boey, F.; Zhang, H. Small 2011, 7, 1876.
(33) Guo, S.; Dong, S. Chem. Soc. Rev. 2011, 40, 2644.
(34) Wei, D.; Liu, Y. Adv. Mater. 2010, 22, 3225.
(35) Liu, H.; Liu, Y.; Zhu, D. J. Mater. Chem. 2011, 21, 3335.
(36) Reina, A.; Jia, X. T.; Ho, J.; Nezich, D.; Son, H.; Bulovic, V.;
Dresselhaus, M. S.; Kong, J. Nano Lett. 2009, 9, 30.
(37) Zhang, J.; Zou, H.; Qing, Q.; Yang, Y.; Li, Q.; Liu, Z.; Guo, X.;
Du, Z. J. Phys. Chem. B 2003, 107, 3712.
(38) Che, G.; Lakshmi, B. B.; Martin, C. R.; Fisher, E. R.; Ruoﬀ, R. S.
Chem. Mater. 1998, 10, 260.
(39) Maldonado, S.; Morin, S.; Stevenson, K. J. Carbon 2006, 44,
(40) Luo, Z.; Lim, S.; Tian, Z.; Shang, J.; Lai, L.; MacDonald, B.; Fu,
C.; Shen, Z.; Yu, T.; Lin, J. J. Mater. Chem. 2011, 21, 8038.
(41) Qu, L.; Liu, Y.; Baek, J. B.; Dai, L. ACS Nano 2010, 4, 1321.
(42) Di, C. A.; Wei, D.; Yu, G.; Liu, Y.; Guo, Y.; Zhu, D. Adv. Mater.
2008, 20, 3289.
(43) Reddy, A. L. M.; Srivastava, A.; Gowda, S. R.; Gullapalli, H.;
Dubey, M.; Ajayan, P. M. ACS Nano 2010, 4, 6337.
(44) Jin, Z.; Yao, J.; Kittrell, C.; Tour, J. M. ACS Nano 2011, 5, 4112.
(45) Imamura, G.; Saiki, K. J. Phys. Chem. C 2011, 115, 10000.
(46) Cho, Y. J.; Kim, H. S.; Baik, S. Y.; Myung, Y.; Jung, C. S.; Kim,
C. H.; Park, J.; Kang, H. S. J. Phys. Chem. C 2011, 115, 3737.
(47) Kudashov, A. G.; Okotrub, A. V.; Bulusheva, L. G.; Asanov, I. P.;
Shubin, Y. V.; Yudanov, N. F.; Yudanova, L. I.; Danilovich, V. S.;
Abrosimov, O. G. J. Phys. Chem. B 2004, 108, 9048.
(48) Liu, J.; Webster, S.; Carroll, D. L. J. Phys. Chem. B 2005, 109,
(49) Lv, W. X.; Zhang, R.; Xia, T. L.; Bi, H. M.; Shi, K. Y. J. Nanopart.
Res. 2011, 13, 2351.
(50) Zhang, C.; Fu, L.; Liu, N.; Liu, M.; Wang, Y.; Liu, Z. Adv. Mater.
2011, 23, 1020.
(51) Choucair, M.; Thordarson, P.; Stride, J. A. Nat. Nanotechnol.
2009, 4, 30.
(52) Deng, D.; Pan, X.; Yu, L.; Cui, Y.; Jiang, Y.; Qi, J.; Li, W. X.; Fu,
Q.; Ma, X.; Xue, Q.; Sun, G.; Bao, X. Chem. Mater. 2011, 23, 1188.
(53) Droppa, R.; Hammer, P.; Carvalho, A. C. M.; dos Santos, M. C.;
Alvarez, F. J. Non-Cryst. Solids 2002, 299−302, 874.
(54) Journet, C.; Maser, W. K.; Bernier, P.; Loiseau, A.; Lamy de la
Chapelle, M.; Lefrant, S.; Deniard, P.; Lee, R.; Fischer, J. E. Nature
1997, 388, 756.
(55) Suenaga, K.; Colliex, C.; Demoncy, N.; Loiseau, A.; Pascard, H.;
Willaime, F. Science 1997, 278, 653.
(56) Panchakarla, L. S.; Subrahmanyam, K. S.; Saha, S. K.;
Govindaraj, A.; Krishnamurthy, H. R.; Waghmare, U. V.; Rao, C. N.
R. Adv. Mater. 2009, 21, 4726.
(57) Ghosh, A.; Late, D. J.; Panchakarla, L. S.; Govindaraj, A.; Rao, C.
N. R. J. Exp. Nanosci. 2009, 4, 313.
(58) Subrahmanyam, K. S.; Panchakarla, L. S.; Govindaraj, A.; Rao,
C. N. R. J. Phys. Chem. C 2009, 113, 4257.
(59) Guo, B.; Liu, Q.; Chen, E.; Zhu, H.; Fang, L.; Gong, J. R. Nano
Lett. 2010, 10, 4975.
(60) Geng, D.; Chen, Y.; Chen, Y.; Li, Y.; Li, R.; Sun, X.; Ye, S.;
Knights, S. Energy Environ. Sci. 2011, 4, 760.
(61) Kinoshita, K. Carbon: Electrochemical and Physicochemical
Properties; Wiley: New York, 1988.
(62) Sheng, Z. H.; Shao, L.; Chen, J. J.; Bao, W. J.; Wang, F. B.; Xia,
X. H. ACS Nano 2011, 5, 4350.
(63) Li, X.; Wang, H.; Robinson, J. T.; Sanchez, H.; Diankov, G.; Dai,
H. J. Am. Chem. Soc. 2009, 131, 15939.
(64) Golberg, D.; Bando, Y.; Bourgeois, L.; Kurashima, K.; Sato, T.
Carbon 2000, 38, 2017.
(65) Morant, C.; Andrey, J.; Prieto, P.; Mendiola, D.; Sanz, J. M.;
Elizalde, E. Phys. Status Solidi A 2006, 203, 1069.
(66) Suenaga, K.; Johansson, M. P.; Hellgren, N.; Broitman, E.;
Wallenberg, L. R.; Colliex, C.; Sundgren, J. E.; Hultman, L. Chem. Phys.
Lett. 1999, 300, 695.
(67) Imran Jafri, R.; Rajalakshmi, N.; Ramaprabhu, S. J. Mater. Chem.
2010, 20, 7114.
(68) Wang, Y.; Shao, Y.; Matson, D. W.; Li, J.; Lin, Y. ACS Nano
2010, 4, 1790.
(69) Jeong, H. M.; Lee, J. W.; Shin, W. H.; Choi, Y. J.; Shin, H. J.;
Kang, J. K.; Choi, J. W. Nano Lett. 2011, 11, 2472.
(70) Lin, Y. C.; Lin, C. Y.; Chiu, P. W. Appl. Phys. Lett. 2010, 96,
(71) Long, D.; Li, W.; Ling, L.; Miyawaki, J.; Mochida, I.; Yoon, S. H.
Langmuir 2010, 26, 16096.
(72) Wang, D. W.; Gentle, I. R.; Lu, G. Q. Electrochem. Commun.
2010, 12, 1423.
(73) Zhang, L. S.; Liang, X. Q.; Song, W. G.; Wu, Z. Y. Phys. Chem.
Chem. Phys. 2010, 12, 12055.
(74) Cançado, L. G.; Pimenta, M. A.; Neves, B. R. A.; Dantas, M. S.
S.; Jorio, A. Phys. Rev. Lett. 2004, 93, 247401.
(75) Dresselhaus, M. S.; Dresselhaus, G.; Saito, R.; Jorio, A. Phys. Rep.
2005, 409, 47.
(76) Ferrari, A. C.; Meyer, J. C.; Scardaci, V.; Casiraghi, C.; Lazzeri,
M.; Mauri, F.; Piscanec, S.; Jiang, D.; Novoselov, K. S.; Roth, S.; Geim,
A. K. Phys. Rev. Lett. 2006, 97, 187401.
(77) Tuinstra, F.; Koenig, J. L. J. Chem. Phys. 1970, 53, 1126.
(78) Nemanich, R. J.; Solin, S. A. Phys. Rev. B 1979, 20, 392.
ACS Catalysis Review
dx.doi.org/10.1021/cs200652y | ACS Catal. 2012, 2, 781−794793
(79) Cançado, L. G.; Takai, K.; Enoki, T.; Endo, M.; Kim, Y. A.;
Mizusaki, H.; Jorio, A.; Coelho, L. N.; Magalhães-Paniago, R.; Pimenta,
M. A. Appl. Phys. Lett. 2006, 88, 163106.
(80) Das, A.; Pisana, S.; Chakraborty, B.; Piscanec, S.; Saha, S. K.;
Waghmare, U. V.; Novoselov, K. S.; Krishnamurthy, H. R.; Geim, A.
K.; Ferrari, A. C.; Sood, A. K. Nat. Nanotechnol. 2008, 3, 210.
(81) Ni, Z. H.; Wang, H. M.; Kasim, J.; Fan, H. M.; Yu, T.; Wu, Y.
H.; Feng, Y. P.; Shen, Z. X. Nano Lett. 2007, 7, 2758.
(82) Graf, D.; Molitor, F.; Ensslin, K.; Stampfer, C.; Jungen, A.;
Hierold, C.; Wirtz, L. Nano Lett. 2007, 7, 238.
(83) Wu, Y. H.; Yu, T.; Shen, Z. X. J. Appl. Phys. 2010, 108, 071301.
(84) Zhao, L.; He, R.; Rim, K. T.; Schiros, T.; Kim, K. S.; Zhou, H.;
Gutiérrez, C.; Chockalingam, S. P.; Arguello, C. J.; Pálová, L.;
Nordlund, D.; Hybertsen, M. S.; Reichman, D. R.; Heinz, T. F.; Kim,
P.; Pinczuk, A.; Flynn, G. W.; Pasupathy, A. N. Science 2011, 333, 999.
(85) Casiraghi, C.; Pisana, S.; Novoselov, K. S.; Geim, A. K.; Ferrari,
A. C. Appl. Phys. Lett. 2007, 91, 233108.
(86) Gupta, A.; Chen, G.; Joshi, P.; Tadigadapa, S.; Eklund, P. C.
Nano Lett. 2006, 6, 2667.
(87) Ferrari, A. C. Solid State Commun. 2007, 143, 47.
(88) Herz, M.; Giessibl, F. J.; Mannhart, J. Phys. Rev. B 2003, 68,
(89) Zheng, B.; Hermet, P.; Henrard, L. ACS Nano 2010, 4, 4165.
(90) Yu, Y. L.; Hu, Y. P.; Liu, X.; Deng, W. Q.; Wang, X. Electrochim.
Acta 2009, 54, 3092.
(91) Sun, S.; Murray, C. B.; Weller, D.; Folks, L.; Moser, A. Science
2000, 287, 1989.
(92) Kristian, N.; Yan, Y. S.; Wang, X Chem. Commun. 2008, 353.
(93) Kristian, N.; Yu, Y. L.; Gunawan, P.; Xu, R.; Deng, W. Q.; Liu,
X. W.; Wang, X. Electrochim. Acta 2009, 54, 4916.
(94) Wang, Y.; Nguyen, T.; Liu, X.; Wang, X. J. Power Sources 2010,
(95) Aihara, J. I. J. Phys. Chem. A 1999, 103, 7487.
(96) Kurak, K. A.; Anderson, A. B. J. Phys. Chem. C 2009, 113, 6730.
(97) Huang, S. F.; Terakura, K.; Ozaki, T.; Ikeda, T.; Boero, M.;
Oshima, M.; Ozaki, J. I.; Miyata, S. Phys. Rev. B 2009, 80, 235410.
(98) Yu, L.; Pan, X.; Cao, X.; Hu, P.; Bao, X. J. Catal. 2011, 282, 183.
(99) Paulus, U. A.; Schmidt, T. J.; Gasteiger, H. A.; Behm, R. J. J.
Electroanal. Chem. 2001, 495, 134.
(100) Nagaiah, T. C.; Kundu, S.; Bron, M.; Muhler, M.; Schuhmann,
W. Electrochem. Commun. 2010, 12, 338.
(101) Niwa, H.; Horiba, K.; Harada, Y.; Oshima, M.; Ikeda, T.;
Terakura, K.; Ozaki, J. I.; Miyata, S. J. Power Sources 2009, 187, 93.
(102) Okamoto, Y. Appl. Surf. Sci. 2009, 256, 335.
(103) Tsai, C. W.; Tu, M. H.; Chen, C.-J.; Hung, T. F.; Liu, R. S.;
Liu, W. R.; Lo, M. Y.; Peng, Y. M.; Zhang, L.; Zhang, J.; Shy, D. S.;
Xing, X. K. RSC Adv. 2011, 1, 1349.
(104) Liang, Y.; Li, Y.; Wang, H.; Zhou, J.; Wang, J.; Regier, T.; Dai,
H. Nat. Mater. 2011, 10, 780.
(105) Avouris, P.; Chen, Z.; Perebeinos, V. Nat. Nanotechnol. 2007,
(106) Schwierz, F. Nat. Nanotechnol. 2010, 5, 487.
(107) Wei, X. L.; Fang, H.; Wang, R. Z.; Chen, Y. P.; Zhong, J. X.
Appl. Phys. Lett. 2011, 99, 012107.
(108) Son, Y. W.; Cohen, M. L.; Louie, S. G. Phys. Rev. Lett. 2006, 97,
(109) Yu, S. S.; Zheng, W. T.; Wen, Q. B.; Jiang, Q. Carbon 2008, 46,
(110) Li, Y.; Zhou, Z.; Shen, P.; Chen, Z. ACS Nano 2009, 3, 1952.
(111) Biel, B.; Blase, X.; Triozon, F.; Roche, S. Phys. Rev. Lett. 2009,
(112) Perebeinos, V.; Tersoﬀ, J.; Avouris, P. Phys. Rev. Lett. 2005, 94,
(113) Zhou, X.; Park, J. Y.; Huang, S.; Liu, J.; McEuen, P. L. Phys.
Rev. Lett. 2005, 95, 146805.
(114) Pan, D.; Wang, S.; Zhao, B.; Wu, M.; Zhang, H.; Wang, Y.;
Jiao, Z. Chem. Mater. 2009, 21, 3136.
(115) Wu, Z. S.; Ren, W.; Xu, L.; Li, F.; Cheng, H. M. ACS Nano
2011, 5, 5463.
(116) Wang, H.; Zhang, C.; Liu, Z.; Wang, L.; Han, P.; Xu, H.;
Zhang, K.; Dong, S.; Yao, J.; Cui, G. J. Mater. Chem. 2011, 21, 5430.
(117) Cho, Y. J.; Kim, H. S.; Im, H.; Myung, Y.; Jung, G. B.; Lee, C.
W.; Park, J.; Park, M. H.; Cho, J.; Kang, H. S. J. Phys. Chem. C 2011,
(118) Jia, L.; Wang, D. H.; Huang, Y. X.; Xu, A. W.; Yu, H. Q. J. Phys.
Chem. C 2011, 115, 11466.
ACS Catalysis Review
dx.doi.org/10.1021/cs200652y | ACS Catal. 2012, 2, 781−794794